General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.77 g/cm³ Show Material materials with Density of 7.77 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 212 - 212.36 GPa Show Material materials with Elastic modulus of 212 - 212.36 GPa |

95.0 °C | 208.22 GPa Show Material materials with Elastic modulus of 208.22 GPa | |

100.0 °C | 207 - 212 GPa Show Material materials with Elastic modulus of 207 - 212 GPa | |

150.0 °C | 204.77 GPa Show Material materials with Elastic modulus of 204.77 GPa | |

200.0 °C | 199 - 205 GPa Show Material materials with Elastic modulus of 199 - 205 GPa | |

205.0 °C | 200.64 GPa Show Material materials with Elastic modulus of 200.64 GPa | |

260.0 °C | 195.81 GPa Show Material materials with Elastic modulus of 195.81 GPa | |

300.0 °C | 192 - 198 GPa Show Material materials with Elastic modulus of 192 - 198 GPa | |

315.0 °C | 191.67 GPa Show Material materials with Elastic modulus of 191.67 GPa | |

370.0 °C | 187.54 GPa Show Material materials with Elastic modulus of 187.54 GPa | |

400.0 °C | 184 - 189 GPa Show Material materials with Elastic modulus of 184 - 189 GPa | |

425.0 °C | 182.71 GPa Show Material materials with Elastic modulus of 182.71 GPa | |

485.0 °C | 177.89 GPa Show Material materials with Elastic modulus of 177.89 GPa | |

500.0 °C | 175 - 180 GPa Show Material materials with Elastic modulus of 175 - 180 GPa | |

540.0 °C | 172.37 GPa Show Material materials with Elastic modulus of 172.37 GPa | |

595.0 °C | 166.85 GPa Show Material materials with Elastic modulus of 166.85 GPa | |

600.0 °C | 164 - 168 GPa Show Material materials with Elastic modulus of 164 - 168 GPa | |

650.0 °C | 159.96 GPa Show Material materials with Elastic modulus of 159.96 GPa | |

705.0 °C | 151.69 GPa Show Material materials with Elastic modulus of 151.69 GPa | |

760.0 °C | 139.27 GPa Show Material materials with Elastic modulus of 139.27 GPa | |

Elongation | 20.0 °C | 18 - 22 % Show Material materials with Elongation of 18 - 22 % |

Elongation, transverse | 20.0 °C | 18 % Show Material materials with Elongation, transverse of 18 % |

Hardness, Brinell | 20.0 °C | 163 - 220 [-] Show Material materials with Hardness, Brinell of 163 - 220 [-] |

Poisson's ratio | 20.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] |

95.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

150.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

205.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

260.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

315.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

370.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

425.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

485.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

540.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

595.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

650.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

705.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

760.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 81.36 GPa Show Material materials with Shear modulus of 81.36 GPa |

95.0 °C | 80.32 GPa Show Material materials with Shear modulus of 80.32 GPa | |

150.0 °C | 78.95 GPa Show Material materials with Shear modulus of 78.95 GPa | |

205.0 °C | 77.22 GPa Show Material materials with Shear modulus of 77.22 GPa | |

260.0 °C | 75.5 GPa Show Material materials with Shear modulus of 75.5 GPa | |

315.0 °C | 73.77 GPa Show Material materials with Shear modulus of 73.77 GPa | |

370.0 °C | 72.05 GPa Show Material materials with Shear modulus of 72.05 GPa | |

425.0 °C | 70.33 GPa Show Material materials with Shear modulus of 70.33 GPa | |

485.0 °C | 67.57 GPa Show Material materials with Shear modulus of 67.57 GPa | |

540.0 °C | 66.19 GPa Show Material materials with Shear modulus of 66.19 GPa | |

595.0 °C | 63.78 GPa Show Material materials with Shear modulus of 63.78 GPa | |

650.0 °C | 60.67 GPa Show Material materials with Shear modulus of 60.67 GPa | |

705.0 °C | 57.23 GPa Show Material materials with Shear modulus of 57.23 GPa | |

760.0 °C | 52.4 GPa Show Material materials with Shear modulus of 52.4 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 410 - 540 MPa Show Material materials with Tensile strength of 410 - 540 MPa |

100.0 °C | 360 MPa Show Material materials with Tensile strength of 360 MPa | |

150.0 °C | 350 MPa Show Material materials with Tensile strength of 350 MPa | |

200.0 °C | 340 MPa Show Material materials with Tensile strength of 340 MPa | |

250.0 °C | 340 MPa Show Material materials with Tensile strength of 340 MPa | |

300.0 °C | 340 MPa Show Material materials with Tensile strength of 340 MPa | |

350.0 °C | 330 MPa Show Material materials with Tensile strength of 330 MPa | |

400.0 °C | 320 MPa Show Material materials with Tensile strength of 320 MPa | |

450.0 °C | 300 MPa Show Material materials with Tensile strength of 300 MPa | |

500.0 °C | 270 MPa Show Material materials with Tensile strength of 270 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 20.0 °C | 395 - 560 MPa Show Material materials with Tensile strength, transverse of 395 - 560 MPa |

Yield strength | 20.0 °C | 175 MPa Show Material materials with Yield strength of 175 MPa |

Yield strength Rp0.2 | 20.0 °C | 175 MPa Show Material materials with Yield strength Rp0.2 of 175 MPa |

100.0 °C | 156 MPa Show Material materials with Yield strength Rp0.2 of 156 MPa | |

150.0 °C | 149 - 150 MPa Show Material materials with Yield strength Rp0.2 of 149 - 150 MPa | |

200.0 °C | 142 - 148 MPa Show Material materials with Yield strength Rp0.2 of 142 - 148 MPa | |

250.0 °C | 138 - 147 MPa Show Material materials with Yield strength Rp0.2 of 138 - 147 MPa | |

300.0 °C | 132 - 145 MPa Show Material materials with Yield strength Rp0.2 of 132 - 145 MPa | |

350.0 °C | 128 - 142 MPa Show Material materials with Yield strength Rp0.2 of 128 - 142 MPa | |

400.0 °C | 125 - 137 MPa Show Material materials with Yield strength Rp0.2 of 125 - 137 MPa | |

450.0 °C | 119 - 129 MPa Show Material materials with Yield strength Rp0.2 of 119 - 129 MPa | |

500.0 °C | 112 - 116 MPa Show Material materials with Yield strength Rp0.2 of 112 - 116 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 175 MPa Show Material materials with Yield strength Rp0.2, transverse of 175 MPa |

100.0 °C | 136 - 156 MPa Show Material materials with Yield strength Rp0.2, transverse of 136 - 156 MPa | |

150.0 °C | 129 - 149 MPa Show Material materials with Yield strength Rp0.2, transverse of 129 - 149 MPa | |

200.0 °C | 122 - 142 MPa Show Material materials with Yield strength Rp0.2, transverse of 122 - 142 MPa | |

250.0 °C | 118 - 138 MPa Show Material materials with Yield strength Rp0.2, transverse of 118 - 138 MPa | |

300.0 °C | 112 - 132 MPa Show Material materials with Yield strength Rp0.2, transverse of 112 - 132 MPa | |

350.0 °C | 108 - 128 MPa Show Material materials with Yield strength Rp0.2, transverse of 108 - 128 MPa | |

400.0 °C | 105 - 125 MPa Show Material materials with Yield strength Rp0.2, transverse of 105 - 125 MPa | |

450.0 °C | 99 - 119 MPa Show Material materials with Yield strength Rp0.2, transverse of 99 - 119 MPa | |

500.0 °C | 92 - 112 MPa Show Material materials with Yield strength Rp0.2, transverse of 92 - 112 MPa | |

Unlock all property charts | ||

Yield strength, transverse | 20.0 °C | 155 - 175 MPa Show Material materials with Yield strength, transverse of 155 - 175 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1E-5 1/K Show Material materials with Coefficient of thermal expansion of 1E-5 1/K | |

20.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | ||

100.0 °C | 1.13E-5 - 1.14E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.13E-5 - 1.14E-5 1/K | ||

200.0 °C | 1.18E-5 - 1.2E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.18E-5 - 1.2E-5 1/K | ||

300.0 °C | 1.23E-5 - 1.24E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.23E-5 - 1.24E-5 1/K | ||

400.0 °C | 1.27E-5 - 1.28E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.27E-5 - 1.28E-5 1/K | ||

425.0 °C | 1.24E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.24E-5 1/K | ||

485.0 °C | 1.26E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.26E-5 1/K | ||

500.0 °C | 1.3E-5 - 1.32E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.3E-5 - 1.32E-5 1/K | ||

540.0 °C | 1.28E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.28E-5 1/K | ||

595.0 °C | 1.29E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.29E-5 1/K | ||

600.0 °C | 1.32E-5 - 1.34E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 - 1.34E-5 1/K | ||

650.0 °C | 1.32E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 1/K | ||

700.0 °C | 1.33E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.33E-5 1/K | ||

705.0 °C | 1.32E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 650 °C Show Material materials with Max service temperature, long of 0 - 650 °C | ||

Melting point | 1382 - 1529 °C Show Material materials with Melting point of 1382 - 1529 °C | Typical for Chromium Molybdenum Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | ||

100.0 °C | 479 - 490 J/(kg·K) Show Material materials with Specific heat capacity of 479 - 490 J/(kg·K) | ||

200.0 °C | 499 - 530 J/(kg·K) Show Material materials with Specific heat capacity of 499 - 530 J/(kg·K) | ||

300.0 °C | 517 - 560 J/(kg·K) Show Material materials with Specific heat capacity of 517 - 560 J/(kg·K) | ||

400.0 °C | 536 - 610 J/(kg·K) Show Material materials with Specific heat capacity of 536 - 610 J/(kg·K) | ||

500.0 °C | 558 - 670 J/(kg·K) Show Material materials with Specific heat capacity of 558 - 670 J/(kg·K) | ||

600.0 °C | 587 - 760 J/(kg·K) Show Material materials with Specific heat capacity of 587 - 760 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 20.3 W/(m·K) Show Material materials with Thermal conductivity of 20.3 W/(m·K) | |

100.0 °C | 22.7 - 23 W/(m·K) Show Material materials with Thermal conductivity of 22.7 - 23 W/(m·K) | ||

200.0 °C | 25 W/(m·K) Show Material materials with Thermal conductivity of 25 W/(m·K) | ||

300.0 °C | 26 - 26.4 W/(m·K) Show Material materials with Thermal conductivity of 26 - 26.4 W/(m·K) | ||

400.0 °C | 27 - 27.3 W/(m·K) Show Material materials with Thermal conductivity of 27 - 27.3 W/(m·K) | ||

500.0 °C | 27.7 - 28 W/(m·K) Show Material materials with Thermal conductivity of 27.7 - 28 W/(m·K) | ||

600.0 °C | 27.8 - 28 W/(m·K) Show Material materials with Thermal conductivity of 27.8 - 28 W/(m·K) | ||

700.0 °C | 27.5 W/(m·K) Show Material materials with Thermal conductivity of 27.5 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | |

100.0 °C | 5.9 mm²/s Show Material materials with Thermal diffusivity of 5.9 mm²/s | ||

200.0 °C | 6.1 mm²/s Show Material materials with Thermal diffusivity of 6.1 mm²/s | ||

300.0 °C | 6 mm²/s Show Material materials with Thermal diffusivity of 6 mm²/s | ||

400.0 °C | 5.8 mm²/s Show Material materials with Thermal diffusivity of 5.8 mm²/s | ||

500.0 °C | 5.4 mm²/s Show Material materials with Thermal diffusivity of 5.4 mm²/s | ||

600.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 5.14E-7 Ω·m Show Material materials with Electrical resistivity of 5.14E-7 Ω·m |

100.0 °C | 5.6E-7 - 5.63E-7 Ω·m Show Material materials with Electrical resistivity of 5.6E-7 - 5.63E-7 Ω·m | |

200.0 °C | 6.3E-7 - 6.32E-7 Ω·m Show Material materials with Electrical resistivity of 6.3E-7 - 6.32E-7 Ω·m | |

300.0 °C | 7.1E-7 - 7.12E-7 Ω·m Show Material materials with Electrical resistivity of 7.1E-7 - 7.12E-7 Ω·m | |

400.0 °C | 7.97E-7 - 8E-7 Ω·m Show Material materials with Electrical resistivity of 7.97E-7 - 8E-7 Ω·m | |

500.0 °C | 8.9E-7 - 8.93E-7 Ω·m Show Material materials with Electrical resistivity of 8.9E-7 - 8.93E-7 Ω·m | |

600.0 °C | 9.96E-7 - 1E-6 Ω·m Show Material materials with Electrical resistivity of 9.96E-7 - 1E-6 Ω·m | |

700.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.06 - 0.15 % Show Material materials with Carbon of 0.06 - 0.15 % |

Chromium | 4 - 6 % Show Material materials with Chromium of 4 - 6 % |

Manganese | 0.3 - 60 % Show Material materials with Manganese of 0.3 - 60 % |

Molybdenum | 0.45 - 0.65 % Show Material materials with Molybdenum of 0.45 - 0.65 % |

Phosphorus | 0.03 - 0.04 % Show Material materials with Phosphorus of 0.03 - 0.04 % |

Silicon | 0.3 - 0.5 % Show Material materials with Silicon of 0.3 - 0.5 % |

Sulfur | 0.03 - 0.035 % Show Material materials with Sulfur of 0.03 - 0.035 % |

Do you have a technical question or need more information about this material?

Post it as a comment below and receive answers from engineers and other community members.